15 342 BRIEF REPORTS PRB 62
FIG. 1. STM image of Sb 1 2 growth on the 2 1 Si(001)
surface at 575 K 0.1 nA, bias referred to substrate Sb lines extend
from two to about 12 dimers 5 nm . Note the splitting of the Sb
dimer row into a ‘‘double’’ line similar to the Si * orbital in the
FIG. 2. STM image of 0.23 ML of Sb on Si 001 at 1.2V subs
empty state image. Most of the Sb dimer rows terminate between
and 0.1 nA annealed at 600 K. The inset shows the upper left region
the chains of the Si. In the schematic the Sb line is shown with
at 1 V. No dark disorder patches are observable as well as no
the two possible termination types: on a former Si dimer row left
chemical contrast. This is consistent with Sb on Si; however, dif-
and between dimer rows right, occurs much more frequently .
ferent from what Garni et al. reported in their Figs. 4 c and 4 d
under similar conditions.
no three-dimensional growth up to the desorption tempera-
ture of the Sb. for 5 min. We speculate that the Sb has desorbed from the
When the surface is annealed at 575 K the Sb orders into surface and is not incorporated into the substrate which is
short lines up to 5 nm orthogonal to the Si dimer rows as consistent with work done by Wasserfall and Ranke.13
shown in Fig. 1. We observe 1 2 epitaxial growth of Sb on We have performed local density of states measurements
the 2 1 reconstructed Si which is consistent with the study of the Sb clusters, lines, and islands by means of scanning
by Richter et al.7 of 820 K annealed Sb layers 0.6 ML and tunneling spectroscopy. The feedback loop is opened after
more , leading to three-dimensional growth. The schematic stabilizing the tunneling gap ‘‘freezing’’ the tip position
in Fig. 1 shows the structure of the Sb2 adsorption and the and we record the current as a function of voltage, I(V).
1 2 growth of the Sb dimer rows. We have varied the Sb2 This is done in a grid of points on the surface and several of
coverage from 1% to 70% and the annealing temperature these curves were averaged at distinct features e.g., Sb2
from 525 to 600 K as well as the annealing time and always dimer .
ﬁnd the same maximum length of Sb lines. Figure 3 shows the spatially resolved density of states of
It is essential to demonstrate that we indeed observe Sb an epitaxial Sb line on Si. This spectroscopy data were taken
structures on Si and not Si on Si. Starting from a low cover- after an anneal at 575 K. These topography of the 3D image
age of Sb Garni et al.9 also observed the formation of dimer reﬂects the constant current scan with several free Sb2
rows on the surface. However, in contrast to our work and dimers and a Sb dimer row. The brightness indicates the
earlier studies they argue that these consist of Si which was density of states at the Fermi level. The area with a ﬁnite
replaced by Sb in the terrace structure at temperatures above density of states is always restricted to the end of Sb lines.
460 K leading to Si2 ad-dimers. The key observations of Ref. The dI/dV spectra of free Sb2 dimers show a gap similar to
9 are the chemical contrast observed at low negative sample Si. The I(V) inset shows the region around the Fermi energy
bias and a high defect density on the Sb:Si 001 surface. We where the ends of the Sb dimer row show a ﬁnite slope in
performed these experiments in the temperature and cover- contrast to the Sb line center and the Si.
age range stated in the previous paragraph and observe no The normalized numerical derivative of the spectroscopy
increase in the number of defects after annealing. Further- data in Fig. 3 is presented in Fig. 4 over the full acquired
more, we observe no chemical contrast: no dark disordered energy range. It shows three distinct classes of curves: ﬁrst,
regions appear when scanning at low bias as shown in Fig. 2. the Sb2 dimer with a low state density near E F and a peak in
Additionally, the observed epitaxial lines are limited to a the LDOS at a valence energy deeper than the Si; second, the
maximum length of 5 nm which is inconsistent with Si on enhanced LDOS near E F 0.5 eV and ﬁnite LDOS at E F for
Si 001 . Much longer epitaxial lines are observed for Si on the Sb-line end; and third, the center of the Sb line with
Si.10 We conclude that we observe Sb2 dimers and dimer almost identical LDOS as the bare Si 001 2 1. Not shown
rows on Si which is consistent with earlier studies.6–8,11,12 in the ﬁgure is spectroscopy averaged over a Sb4 cluster.
Further annealing of the sample at 700 K leads to the Spectroscopy curves of Sb4 clusters display very little struc-
conversion of the Sb dimer rows to islands. The amount of ture and are lower in amplitude compared to the Si and the
Sb on the surface does not change during the conversion of other Sb structures. This may be attributed to weak bonding/
Sb2 dimers to the islands. This was conﬁrmed by annealing a coupling to the substrate of this nonepitaxial cluster. The
sample with a certain Sb coverage from free Sb dimers to Sb results demonstrate a signiﬁcant change of the observed
dimer rows and then to the Sb islands while analyzing the Sb LDOS when the Sb2 is incorporated in a Sb dimer row.
surface coverage in the STM images. The maximum length The Si 001 2 1 surface shows the bonding and anti-
of Sb rows in these islands is about 8 nm which is consider- bonding * state as shown clearly in Fig. 4. The observa-
ably longer than the Sb lines with a maximum of 5 nm. A tions conﬁrm the identical behavior of the center of the Sb
clean 2 1 Si surface reestablishes after an anneal at 775 K line and the Si in contrast to the end state which peaks closer
PRB 62 BRIEF REPORTS 15 343
FIG. 3. Color Epitaxial Sb line on Si 2
1. The apparent height reﬂects the topography
at 2V sam ple and the color the magnitude of
dI/dV at 0 V as shown in the I(V) inset from
blue over red to white for 0 to 2pA/V). Only the
ends of the Sb line show a ﬁnite density of states
at the Fermi level marking the reactive sites of
the surface polymerization in contrast to the free
Sb2 dimers the two dimers on the upper left are
separated by a * chain and not bonded like a Sb
line . The vertical scale is exaggerated, the Sb2
dimers and Sb line appear as 0.1 nm features in
to the Fermi level. It is interesting to note that the Sb lines the growth kinetics. We think that the ﬁndings for Si on
show a more pronounced * -like feature than the Si which Si 001 must be attributed to a similar origin as for Sb on
is consistent with the clear antibonding like character of the Si 001 . The 1D growth of Sb on Si 001 is based on the
Sb line as shown in the empty state image of Fig. 1. This is higher probability of an ad-dimer to stick to the end of the Sb
surprising since one could expect an occupied * orbital line versus the side of the line. The observation of a ﬁnite
when the lone pairs of the Sb atoms hybridize. Thus, the density of states at the Fermi level uniquely links the growth
state we observe is most likely not just a * state but a mode to the microscopic electronic properties of the struc-
different antibonding orbital of the complicated Sb on the Si ture.
system. The ends of the Sb line show a ﬁnite density of states The reactive end is the nucleation site for the next build-
at E F but we still observe a peak in the LDOS at ing block of the polymer chain as shown in the schematic of
0.5 eV. We speculate that this may be due to the interac- Fig. 1 at, e.g., the left end of the Sb line. A Sb2 dimer can
tion between the two dangling bonds of the reactive site. bond to the two dangling bonds and extend the chain by
A central result of the spectroscopy work is the observa-
breaking the bond of the next Si2 dimer. The next step is
tion of a ﬁnite density of states at the Fermi level for the ends
identical to an addition on the right end of the Sb line in Fig.
of the Sb dimer rows. A ﬁnite density at the Fermi level is
the signature of a reactive site like a dangling bond. A dan- 1 where the strained bond needs to be broken to add a
gling bond is half ﬁlled and so is expected to result in a ﬁnite dimer to the Sb line. The process then repeats until the added
slope of the I(V) curve at zero bias ﬁnite LDOS . To our strain discussed below in the Sb line is larger than the gain
knowledge this is the ﬁrst direct observation of the reactive in energy due to the bonding.
end of a structure leading to surface polymerization as pre- The existence of the end state does not depend on the total
dicted by Brocks et al. Ganz et al. studied the 1D growth of length of the Sb line as we have observed in Sb lines ranging
Si on Si 001 and speculated that ‘‘sticky ends’’ may be from two to a maximum length of about 12 Sb2 dimers. We
responsible for the unexpected growth direction and studied ﬁnd the crossover from single dimer behavior abruptly at the
shortest possible ‘‘Sb line’’ with two dimers where one is
located between the chains of the Si. A two dimer Sb line
already shows the end-state behavior which is consistent
with the reactive sites shown for the four dimer Sb line in
The Sb dimer rows preferentially terminate between the
Si chains as shown in Fig. 1 resulting in an odd number of
Sb2 dimers in most of the Sb lines. Apparently this conﬁgu-
ration right end in Fig. 1 is more favorable since the next
growth step would require the break of the bond of the Si2
dimer in the next chain which is probably already strained
but not broken. In the empty state image of Fig. 1 some of
the Sb row ends show a rounded feature which seems to
extend the Sb line partly into the next chain of the Si. We
speculate that this may be an impurity atom, terminating the
FIG. 4. The normalized spectrum (dI/dV)/(I/V) showing simi- reactive end of the Sb line.
lar behavior of the center of the Sb line and the clean Si surface. In contrast to Sb lines of two dimers or more a single Sb2
The Sb line end displays a ﬁnite LDOS at E F and peaks between E F could be bonded via the orbital of the Si 2 1 reconstruc-
and the Si state. tion leaving the Si dimer bond intact. The alternative is the
15 344 BRIEF REPORTS PRB 62
breakup of the bond even for a free dimer. To our knowl- growth. It is necessary to include the energy gain of bonding
edge this question has not been addressed carefully. Our an additional dimer to the Sb line to explain the extended
spectroscopy data show the similarity of the Sb2 states to the growth.
Si2 orbitals, only 0.2 eV shifted to lower valence energy. In conclusion, we presented spectroscopy data on epitax-
Since we observe states at relative low energy 2 eV this ial Sb nanostructures on Si 001 . The ends of the Sb dimer
suggests that the remaining two electrons per Sb atom are row show a ﬁnite density of states at the Fermi level in
not involved in a like bond to the Si leaving the Si-Si contrast to the center of the Sb line which is semiconducting
bond intact. Based on this observation we propose that the with characteristics similar to Si 001 2 1. We found no
Sb2 is chemisorbed by breaking only the bond of the Si2 evidence for the replacement of Si by Sb in the surface. We
dimer. propose that the end state is the experimental evidence for
When a Si 001 surface with Sb2 dimers is annealed at the surface polymerization model.1 The self-assembly of the
sufﬁciently high temperature we achieved this at approxi- Sb line begins by breaking the bond of the Si and a very
mately 575 K the bond of the Si dimer is deﬁnitely reactive site is formed. This site enhances the density of
broken7 and the growth of the Sb dimer row continues until states at E F Fermi level and propagates the surface poly-
it is terminated by strain induced in the Sb line. At lower merization.
temperatures the Sb2 is diffusing on the surface by bonding
to the orbitals. The higher temperature makes it possible to The authors wish to thank T.M. Klapwijk for detailed
break the bond resulting in the reactive ends leading to the discussions concerning this work and J.E. Mooij, S. Rade-
one-dimensional growth discussed here. Considering the ra- laar, and F. Tuinstra for their support. This work was ﬁnan-
tio of the covalent radii of Sb and Si, r Sb /r Si 1.21, 14 it is cially supported by the university and the ‘‘Stichting voor
quite remarkable that the epitaxial Sb lines of Sb grow up to Fundamenteel Onderzoek der Materie FOM ’’ which is a
a maximum length of approximately 5 nm considering the subsection of the ‘‘Nederlandse Organisatie voor Weten-
strain of l/l 17% in the Sb line corresponding to ap- schappelijk Onderzoek NWO .’’ S.R. and L.J.G. wish to
proximately two atoms over 5 nm . This shows that the acknowledge ﬁnancial support from the Royal Netherlands
simple covalent radius model is not sufﬁcient to explain the Academy of Arts and Sciences.
G. Brocks, P. Kelly, and R. Car, Phys. Rev. Lett. 70, 2786 1993 . 1991 .
M. Crommie, C. Lutz, and D. Eigler, Science 262, 218 1993 . B. Garni, I. Kravchenko, and C. Salling, Surf. Sci. 423, 43
3 ´ ´
M. Gonzalez-Mendez and N. Takeuchi, Phys. Rev. B 58, 16 172 1999 .
1998 . C. Pearson, M. Krueger, and E. Ganz, Phys. Rev. Lett. 76, 2306
O. Albrektsen, H. Salemink, K. Morch, and A. Tholen, J. Vac. 1996 .
Sci. Technol. B 12, 3187 1994 . H. Elswijk and E. van Loenen, Ultramicroscopy 42-4, 884 1992 .
S. Barnett, H. Winters, and J. Greene, Surf. Sci. 165, 303 1986 . M. Mendez and N. Takeuchi, Surf. Sci. 432, 239 1999 .
Y. Mo, Phys. Rev. Lett. 71, 2923 1993 . J. Wasserfall and W. Ranke, Surf. Sci. 331-3, 1099 1995 .
M. Richter et al., Phys. Rev. Lett. 65, 3417 1990 . L. Pauling, The Nature of the Chemical Bond Cornell University
J. Nogami, A. Baski, and C. Quate, Appl. Phys. Lett. 58, 475 Press, Ithaca, New York, 1960 .